The adsorption of HCrO4− on activated carbon of date pits and its photoreduction on the hetero-system ZnCo2O4/TiO2
- 647 Downloads
The adsorption properties of activated carbon were successfully tested toward the elimination of hazardous HCrO4− (30, 50, 70 and 100 mg L−1). The material was prepared from Algerian date pits by physical and chemical activations of ZnCl2/CO2 in the goal to develop the microporous volume. The characterization by N2 adsorption at 77 K, the mercury intrusion porosimetry and scanning electron microscopy showed important textural properties. CO2 increases the specific surface area (1192 m2 g−1) and pore volume (0.96 cm3 g). The HCrO4− adsorption is described by a pseudo-first-order kinetic model, and the equilibrium data are fitted by the Langmuir model with a maximal adsorption capacity of 46.72 mg/g within 30 min and a constant KL (0.12 L g−1). The remaining HCrO4− concentrations (8, 23, 32.5 and 43.5 mg L−1) were photocatalytically reduced on the hetero-system ZnCo2O4/TiO2 down to 5 mg L−1. The spinel ZnCo2O4, prepared by co-precipitation from the nitrates precursors and characterized by photoelectrochemistry, gives a conduction band of − 1.49 VSCE, more cathodic than the HCrO4− level (0.53 V). Therefore, the photoelectrons transfer toward HCrO4− species is achieved through TiO2 located midway between the spinel and chromate levels. The photocatalysis is investigated by varying the catalyst dose and HCrO4− concentration. ZnCo2O4 has a gap of 1.82 eV and the best reduction efficiency (82%) was obtained under visible light (50 mW cm−2) and optimal conditions (HCrO4− 23 mg L−1, pH ~ 7, ZnCo2O4/TiO2 50/50%) and follows a first-order kinetic with a rate constant of 3.86 × 10−3 min−1.
KeywordsDate pits Chemical and physical activation Adsorption Chromate Photoreduction Hetero-system ZnCo2O4/TiO2
In the water treatment for the potable water production, the adsorption on activated carbons remains an attractive challenge for the environmental protection. Activated carbon (AC) is composed of a substantially amorphous carbon material (Bansal et al. 1988; Bouchemal et al. 2012; Tawfik Saleh 2015), delivering highly porous texture, a large specific surface area, a good adsorption capacity and a thermal stability (Skodras et al. 2008; Li et al. 2013; Alswat et al. 2016). Recent developments in the physical adsorption have highlighted the applications of AC. In this regard, the adsorption of gases (Wang et al. 2012; Abiko et al. 2010; Balarak et al. 2017), the uptake of organophosphorus pollutants (Jayson et al. 1982), the retention of bacteriologic pollutants in aqueous electrolytes (Oya et al. 1993), the elimination of heavy metals (Lu et al. 2014; Gomez-Eyles et al. 2013) and chromate photoreduction (Dermèche et al. 2017) are mainly documented in the open literature. AC is also used in bleaching and deodorization of certain liquids and can further play a role as catalyst support in heterogeneous catalysis (Polcaro et al. 1993; Qi et al. 2012). As the water quality is more stringent by the World Health Organization, an increased interest was focused on adsorbents (Ghasemian et al. 2015), zeolites (Mekatel et al. 2015; Lemraski and Palizban 2015), clays (Boutra et al. 2017) and activated carbons (Belhamdi et al. 2016; Merzougui et al. 2011) which are widely summarized in review articles. The porosity of AC is crucial for the adsorption and remains improperly explored; it is developed after pyrolysis of the carbon precursor under inert atmosphere. Thus, the adsorption capacity is usually insufficient for the utilization to which it was designated and developing the porous texture of AC remains a priority goal. So, the first part of our work is devoted to the influence of chemical and physical activations using ZnCl2 and CO2 flow on the porous texture of AC obtained from Algerian dates pits. The elaboration of activated carbons is applied for the elimination of inorganic pollutants. In this respect, Cr(VI) is a hazardous compound, selected for the pollution tests, in aqueous media for the adsorption on AC. Chromate comes mainly from tanneries, plating and battery factories and gives rise to large-scale pollution. Therefore, the second part of the work aims at determining the water decontamination by photocatalysis (Saleh and Gupta 2012; Gupta et al. 2012). Indeed, the adsorption yield increases the abatement but becomes inefficient at low concentrations. At this level, the photocatalysis is a clean alternative for the water decontamination which reduces the chromate ions to less harmful forms (Cr3+) by photoelectrons (Rekhila et al. 2016). In this regard, the semiconductors with medium forbidden band are promising for the exploitation of a large part of the solar energy (Rekhila et al. 2013). The study focuses on the HCrO4− reduction under visible light on the hetero-system ZnCo2O4/TiO2. The charge transfer occurs iso-energetically and TiO2 acts a bridge between the conduction band (CB) of ZnCo2O4 and adsorbed HCrO4− ions. Nano-crystallites produce larger active surface areas with more photoelectrochemical sites, and the spinel ZnCo2O4 was prepared by chemical route at lower temperatures. It was selected because of its low cost, light absorption in the visible region and environmentally friendly characteristics (Guo et al. 2014).
Preparation of activated carbons (AC)
Date pits (origin Algeria) are used for the preparation of activated carbons AC. At first, the stones were thoroughly washed with distilled water and dried in an air oven at 120 °C; such protocol was effective to facilitate crushing and grinding. A fraction particle size of between 0.5 and 1 mm was used for the preparation of activated carbons. AC prepared by combining physical and chemical activations was referred in the text as DZCO2: The precursor was impregnated with 7.32 mmol of ZnCl2 as chemical adjuvant in a solid form and then pyrolyzed at 800 °C (heating rate of 5 °C/min) under low N2 flow, followed by physical activation (800 °C) under CO2 flow (20 L h−1, 1 h) and cooled to room temperature. The sample was treated by HCl solution (0.1 M) under reflux ebullition (150 °C, 3 h) in order to eliminate the alkaline compounds and adjuvant excess. DZCO2 was recovered by filtration and thoroughly washed with distilled boiling water until the AgNO3 test on the filtrate became negative. Finally, DZCO2 was dried in air oven at 120 °C (24 h) and stored in glass bottles until use.
The specific surface area was determined with a Micrometrics ASAP 2010 equipment at 77 K. Before measurement, the powder was degassed under vacuum (150 °C, 12 h). The morphology of DZCO2 was studied by scanning electron microscopy (SEM) using a JEOL, JSM-6360LV microscope.
The HCrO4− stock solution (1 g L−1) was prepared by dissolving the accurate amount of K2Cr2O7 (Merck, 99%) in distilled water. The solutions with initial concentrations Co (30, 50, 70 and 100 mg L−1) were made up by dilution. Batch adsorption tests were carried out in 100-mL Erlenmeyer flasks placed in a thermostat shaker bath at 25 °C for 2 days. The adsorption study was realized at natural solution without any pH adjustment in order to avoid the interferences.
The second part was devoted to the HCrO4− reduction under visible light on the hetero-system CoZn2O4/TiO2. The spinel ZnCo2O4 was prepared by co-precipitation; stoichiometric amounts of Co(NO3)2·5H2O (purity 99%, Merck) and Zn(NO3)2·6H2O (99%, Prolabo) were dissolved in distilled water. The solution was evaporated on a hot plate and heated at 150 °C for the nitrate decomposition until disappearance of brown NOx fumes. Then, the powder was ground in an agate mortar and reheated in a programmed furnace at 650 °C (10 °C min−1, 16 h) with three intermediate regrindings. TiO2 (99%) was supplied by Merck company. The phases were identified by X-ray diffraction (XRD) with a Mini-Diffractometer MD-10 using Cu Kα anticathode (λ = 0.15418 nm).
The forbidden band (Eg) was determined from the diffuse reflectance using a dual-beam spectrophotometer (Specord 200 Plus), and PTFE was used as standard. The point of zero charge (pzc) was simply obtained from the equilibrium pH of aqueous solution containing an excess of TiO2 powder using a digital pH meter (Schott CG 825).
The photoelectrochemical (PEC) study was performed in a conventional cell using Pt as auxiliary electrode. The electrical contact on the back pellet was made with silver paint. The electrode surface of the pellet sintered at 700 °C was polished with emery paper (grade 80). The potential of ZnCo2O4 was monitored by PGZ301 potentiostat (Radiometer analytical) and given against a saturated calomel electrode (SCE). The Mott–Schottky characteristic was plotted at a frequency 10 kHz.
The photocatalytic device was composed by a Pyrex reactor open to atmosphere; the temperature was fixed at 25 °C thanks to a thermostated bath. The catalyst powder (100 mg) was suspended in 100 mL of HCrO4− solution at different concentrations (8, 23, 32.5 and 43.5 mg L−1) at natural pH (~ 7). The Erlenmeyers were maintained in the dark overnight and then exposed to visible light under magnetic agitation (400 rpm); the light intensity (mW cm−2) was measured by a flux meter, and the concentration was determined as above.
Results and discussion
Characterization of activated carbons (DZCO2)
The textural characteristics of DZCO2 gave a specific surface area of 1192 m2 g−1 from the BET method through the N2 adsorption isotherms. The mesoporous (Vmeso, ∅ = 3.7–50 nm), macroporous (Vmacro, ∅ > 50 nm) and microporous volumes (Vmicro, ∅ < 3.7 nm) were obtained from mercury intrusion porosimetry. The elemental analysis of the spinel confirmed the presence of Zn, Co and O. The crystallite size of ZnCo2O4 (L ~ 45 nm) was evaluated from the full width at half maximum (FWHM).
Adsorption of chromate under static conditions on AC
The charge transfer in heterogeneous system occurs between levels of similar energy, and TiO2 is used to mediate the electrons transfer since its conduction band is located midway between ZnCo2O4-CB and HCrO4−. Coupled semiconductors improve the separation of (e−/h+) pairs by synergetic effect and shift the spectral photoresponse toward longer wavelengths. Nano-crystallites of ZnCo2O4 prepared by chemical route give large active surface areas and more photocatalytic sites. ZnCo2O4 was chosen because of its light absorption over the visible region and chemical stability.
This paper has given an overview on the preparation, characterization and application of adsorbent material based on activated carbon from date pits for the treatment of water polluted by chromate. We emphasized that the development of the porous texture of the activated carbon prepared by combined activations depends mainly on the nature of the adjuvant. The HCrO4− adsorption of chromate on prepared adsorbent was carried out in a batch reactor, and the data were well filled by the Langmuir isotherm, while the adsorption kinetic followed a pseudo-first-order model. The remaining concentrations remain above the thresholds required by the water standard. Accordingly, the photoelectrochemical HCrO4− reduction is reported on the hetero-system ZnCo2O4/TiO2 to lower the concentration. The decay in the HCrO4− absorbance is attributed to visible light reduction since no change was observed in the dark. The photocatalysis was optimized with respect to the ZnCo2O4 dose and HCrO4− concentration, and a conversion of 82% was obtained.
The activation energy (Ea ~ 0.07 eV) was determined from the electrical conductivity measurement on sintered pellet.
- Bansal RC, Donnet JB, Stoeckli F (1988) Active carbon. Marcel Dekker, New YorkGoogle Scholar
- Boutra B, Trari M, Nassrallah N, Bellal B (2017) Adsorption and photodegradation of solophenyl red 3BL on nanosized ZnFe2O4 under solar light. Theoret Exp Chem 197:490–497Google Scholar
- Charlot G (1961) Les Méthodes de la chimie analytique: analyse quantitative minérale. Masson, ParisGoogle Scholar
- Li ZJ, Shi BY, Wang DS (2013) Comparative study on adsorption behaviors of natural organic matter by powered activated carbons with different particle sizes. Huan Jing Ke Xue 34:4319Google Scholar
- Oya A, Yoshida S, Abe Y, Lizuka T, Makiyama N (1993) Preparation of pitch-based antibacterial activated carbon fiber. Carbon 31:77Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.